JORGE FERNANDO M ´
The effect of biodeterioration on the mechanical
properties of cement mortar
A dissertation by
JORGE FERNANDO M ´ARQUEZ-PE ˜NARANDA
Submitted to School of Engineering, of UNIVERSIDAD DE LOS ANDES
in partial fulfillment of the requirements for the degree of DOCTOR OF PHILOSOPHY
Chair of Committee, Mauricio S´anchez-Silva Committee Members, Johana Husserl
Emilio Bartidas-Arteaga Franck Schoefs
Andr´es Fernando Guzm´an-Guerrero Vice Chancellor of Research, Silvia Restrepo Restrepo
Universidad de los Andes School of Engineering
Carrera 1E. 19A-40 Edicio Mario Laserna
©2017 Jorge Fernando M´arquez-Pe˜naranda ISBN: xxx-xxxx-xx-x
Printed in Colombia Bogot´a 2017
Phone: Fax: Email: http:
Ang´elica Mar´ıa y
I want to thank to my principal advisor Dr. Mauricio S´anchez-Silva for his valuable and wise guide.
To Dr. Johana Husserl, my eternal gratitude for leading me rightly through new concepts.
My deferential recognition to Emilio Bastidas-Arteaga for his permanent professional and personal support.
To Franck Schoefs my appreciation for his ideas of aperture.
Also I want to thank to the fellow doctoral students from the Universidad de los Andes and Universit`e de Nantes, their fresh and opportune help.
To the Universidad de los Andes and Universit`e de Nantes my special gratitude for gathering all the possibilities for my professional and personal development through new experiences.
Many thanks to engineer Joachim Marais at the Institut Universitaire de Technologie (IUT de Nantes/Carquefou) of the Universit`e de Nantes for his valuable helpful in the study of the topographic changes of the samples. I want to thank to Michael O’Byrne, PhD Candidate of the Department of Civil, Structural and Environmental Engineering (Trinity College Dublin) for his collaboration in the determination of volume of samples using video technics.
I am highly grateful to Universidad Francisco de Paula Santander for its financial and academic support.
To my wife and daughters, the best of my feelings for their unconditional love and company.
The following publications are based on this research:
Papers in refereed journals
M´arquez-Pe˜naranda J, S´anchez-Silva M, Husserl J, Bastidas-Arteaga E. Effects of biode-terioration on the mechanical properties of concrete. Materials and Structures. Published on line:29 December 2015. DOI 10.1617/s11527-015-0774-4
M´arquez-Pe˜naranda J, S´anchez-Silva M, Husserl J, Bastidas-Arteaga E. Influence of biodeterioration in structural design of reinforced concrete sewers. In process.
Papers in conferences
M´arquez-P J, S´anchez-Silva M, Husserl J. Review of reinforced concrete biodeterioration mechanics. In: VIII International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS-8. Spain 2013. p. 2088-2096.
M´arquez-P J, S´anchez-Silva M, Husserl J. Biodeterioration of Portland Cement Mortar Produced by Sulfur Oxidizing Bacteria. In: Pipelines 2014: From Underground to the Forefront of Innovation and Sustainability. USA 2014. p. 1568-1577
Reinforced concrete (RC) is the hybrid material most used in construction worldwide and its importance in modern engineering is paramount. Thus, to evaluate its lifecycle performance, it is important to understand the RC behavior under adverse environmen-tal conditions. In particular, this work addresses the problem of concrete deterioration over time as a result of microbial attack. In this document, there is a description of novel experimental work directed to determine the effect of microbial attack on both physical and mechanical concrete properties. Also a proposal to take the biodeteriora-tion effects into account in real structural design situabiodeteriora-tions is presented.
The experimental work was conducted on a set of 13 mm x 13 mm x 10 mm mor-tar Portland type I cement that were inoculated with Hallothiobacillus neapolitanus
NCIMB 8454 (H.n.) andAcidithiobacillus thiooxidans NCIMB 9112 (A.t.) using asep-tic and non asepasep-tic condition. Samples were exposed in two different experiments to peaks of 131 and 222 ppmvH2S, 0.3±0.1%CO2, for 300 and 153 days respectively. The analysis of porosity and strength changes in cement mortar from biodeterioration is a novel contribution of this study. Changes in porosity using mercury intrusion porosime-try, compressive strength and dry weight were measured. Total porosity loses up to 32% and 13% were observed after exposition of inoculated samples and non-inoculated sam-ples, respectively. Major changes were observed in pore-sizes between 10 nm and 5000 nm, slightly smaller changes in pore sizes larger than 5000 nm and no changes in pores smaller than 10 nm. Inoculated samples showed a pronounced strength and weight loss after five months of exposition to bacteria compared to non-inoculated samples.
Previous findings and others reported in the literature were used to propose some considerations as to how to include biodeterioration into concrete design practice. To do so, probability of failure curves were fit from a model based on results obtained from a Matlabr code designed to run the structural analysis and simulate the Montecarlo’s method simustaneously.
El concreto reforzado (RC) es el material h´ıbrido m´as usado a nivel mundial en la construcci´on. Su importancia en la ingenier´ıa moderna es innegable. Por ello, entender su comportamiento bajo condiciones ambientales adversas es clave para comprender su desempe˜no durante su vida ´util. Este trabajo se enfoca en el problema del deterioro del concreto producido por ataque microbiano a trav´es del tiempo (biodeterioro). En este documento se presenta una descripci´on de un trabajo experimental novedoso dirigido a determinar el efecto del ataque microbiano sobre las propiedades fsicas y mecnicas del concreto. Tambi´en se presenta una propuesta para tomar en cuenta el efecto del biodeterioro en situaciones reales de dise˜no.
El trabajo experimental us´o muestras de 13 mm x 13 mm x 10 mm fabricadas con mortero de cemento Portland tipo I que fueron inoculadas con bacterias Halloth-iobacillus neapolitanus NCIMB 8454 (H.n.) y Acidithiobacillus thiooxidans NCIMB 9112 (A.t.) en condiciones as´epticas y no as´epticas. Las muestras fueron expuestas a picos de 131 y 222 ppmvH2S,0.3±0.1%CO2 durante 300 y 153 d´ıas respectivamente Un aporte novedoso de este estudio es la determinaci´on de los cambios de porosidad y resistencia producidos por el biodeterioro en el mortero de cemento. Cambios de porosidad usando t´ecnicas de porosimetr´ıa por intrusion de mercurio, cambios en la resistencia a la compressi´on y cambios en el peso seco de las muestras fueron medidos para las muestras. Despu´es de la exposici´on, valores de porosidad total hasta de 32% y 13% fueron registrados en muestras inoculadas y no inoculadas respectivamente. Los cambios m´as pronunciados se observaron en tama˜nos de poro comprendidos entre 10 nm y 5000 nm, menores cambios en poros ms grandes que 5000 nm y cambios despre-ciables en poros m´as peque˜nos que 10 nm. Despu´es de cinco meses de exposici´on las muestras inoculadas mostraron una importante p´erdida de resistencia y de peso.
Los hallazgos de este estudio en conjunto con los de otros estudios previos se usaron para proponer algunas consideraciones sobre c´omo puede incluirse el biodeterioro en la pr´actica del dise˜no estructural del concreto reforzado. Para hacer esto, se ajustaron curvas de probabilidad de falla a partir de un modelo basado en los resultados obtenidos de un c´odigo Matlabr dise˜nado para ejecutar simult´aneamente el an´alisis estructural y el m´etodo de Montecarlo.
List of Figures xxi
List of Tables xxvii
1 INTRODUCTION 1
1.1 Description of the problem . . . 1
1.2 Background of biodeterioration . . . 2
1.3 Research objectives . . . 3
1.4 Thesis organization . . . 4
2 FUNDAMENTALS OF BIODETERIORATION 7 2.1 Chapter overview . . . 7
2.2 Importance of the biodeterioration effects upon infrastructure systems . 8 2.3 Consequences of biodeterioration . . . 9
2.3.1 Effects on concrete properties . . . 9
2.3.2 Effects on chloride ingress . . . 11
2.4 Biodeterioration in sewers . . . 11
2.4.1 Chemical and biological deterioration in sewers . . . 11
2.4.2 Sewer environment conditioning for biodeterioration . . . 13
2.4.3 Bacteria species related to concrete biodeterioration . . . 13
2.5 Summary and conclusions . . . 15
3 EXPERIMENTAL SETUP 17 3.1 Chapter Overview . . . 17
3.2 Basic principles of the experiment . . . 18
3.3 Culture growth and inoculation of mortar samples . . . 21
3.3.1 Inoculation of OM samples in non aseptic conditions . . . 24
3.3.2 Inoculation of OM samples in aseptic conditions . . . 25
3.3.3 Inoculation of PM samples in non aseptic conditions . . . 25
3.4.2 Pyritic mortar samples (PM) . . . 28
3.4.3 Mortar samples added with Triclosan (TM) . . . 31
3.5 Carbonation of samples . . . 31
3.6 H2S generation and sulfur availability . . . 32
3.7 Exposure of samples to bacterial attack . . . 40
3.7.1 Exposure of OM samples inoculated in non aseptic conditions . . 40
3.7.2 Exposure of OM samples inoculated in aseptic conditions . . . . 40
3.7.3 Exposure of PM samples inoculated in non aseptic conditions . . 41
3.7.4 Exposure of TM samples inoculated in aseptic conditions . . . . 42
3.8 Assessment of physical and mechanical consequences of biodeterioration 42 3.8.1 Weight loss . . . 43
3.8.2 Porosity . . . 44
3.8.3 Compressive strength . . . 45
3.8.4 Volumetric measurements . . . 47
3.9 Determination of chemical compounds in biodeteriorated samples . . . . 48
3.10 Summary and conclusions . . . 48
4 SULFUR AVAILABILITY AND QUALITATIVE CHANGES 51 4.1 Chapter overview . . . 51
4.2 Qualitative changes in biodeteriorated samples . . . 53
4.3 Topographic variations in surfaces of biodeteriorated samples inoculated in aseptic conditions . . . 59
4.4 Chemical compounds in exposed ordinary mortar samples . . . 65
4.5 Volumetric variations in biodeteriorated samples . . . 70
4.6 Summary and conclusions . . . 71
5 BIODETERIORATION EFFECTS UPON PHYSICAL AND ME-CHANICAL PROPERTIES OF MORTAR 73 5.1 Chapter overview . . . 73
5.2 Weight variations in biodeteriorated samples . . . 74
5.3 Porosity variations in biodeteriorated samples . . . 89
5.4 Compressive strength variations in biodeteriorated samples . . . 116
5.5 Strength-porosity relationship in biodeteriorated samples . . . 130
5.6 Summary and conclusions . . . 136
6 PROVISIONS TO CONTROL BIODETERIORATION IN STRUC-TURAL DESIGN OF RC SEWERS 139 6.1 Introduction . . . 139
6.2 Current practice in structural design of sewers . . . 141
6.3 Biodeterioration effects upon reinforced concrete sewers . . . 146
6.4 Consideration of biodeterioration effects in structural design of sewers . 152 6.5 Numerical application . . . 157
6.6 Proposal of methodology for considering biodeterioration effects in struc-tural design of sewers . . . 159 6.7 Conclusions and recommendations for future work . . . 162
7 CLOSURE 165
7.1 Conclusions . . . 165 7.2 Recommendations for future work . . . 168
ASOM Acidophilic Sulfur Oxidizing Microorganisms
A.t. It refers to: a)Acidithiobacillus thiooxidans bacteria. b) Set of samples inoc-ulated in aseptic conditions withA. thiooxidans grown in SM
At Set of samples inoculated in non aseptic conditions withA. thiooxidans grown in SM
Ats Set of samples inoculated in non aseptic conditions withA. thiooxidans grown in MM
Cons. Set of samples inoculated in aseptic conditions with H. neapolitanus and A. thiooxidans grown separately in SM
C-S-H Calcium silicate hydrate (3CaO2SiO24H2O)
ctrl Set of abiotic samples used as control when studying effects related to bacteria inoculated in aseptic or non aseptic conditions
ESVR Exposed surface/volume ratio (mm2/mm3)
H.n. It refers to: a) Hallothiobacillus neapolitanus bacteria. b) Set of samples inoculated in aseptic conditions with H. neapolitanus grown in SM
Hn Set of samples inoculated in non aseptic conditions withH. neapolitanusgrown in SM
Hns Set of samples inoculated in non aseptic conditions withH. neapolitanusgrown in MM
MICC Microbial induced concrete corrosion
MM Seawater (salty) modified liquid medium (DSMZ 68 or DSMZ 35) for H.n. or A.t. growth
NSOM Neutrophilic Sulfur Oxidizing Microorganisms
nt Set of samples inoculated in non aseptic conditions withH. neapolitanus and
A. thiooxidans grown separately in SM
nts Set of samples inoculated in non aseptic conditions withH. neapolitanus and
A. thiooxidans grown separately in MM OD Optical density
OM Ordinary mortar samples pH Potential of hydrogen PM Pyritic mortar samples ppmv Parts per million in volume
SM Standard liquid medium (DSMZ 68 or DSMZ 35) for H.n. or A.t. growth SOB Sulfur oxidizing bacteria
SRB Sulfur reducing bacteria
As Initial rebar area (m2)
Asr Reduced rebar area due to corrosion (m2)
As Spread wheel load area at the outside top of the pipe (m2)
Aw Wheel contact area (m2)
b Cross section width (m) for structural analysis of the pipe
B Trench width (m)
c Extreme fiber to rebar center distance (cm)
C Trench load coefficient
d Internal lever arm of the pipe section (m)
do Available inner lever arm (m) at timeτ = 0
db Mean bar diameter (m)
d(τ) Available inner lever arm (m) at timeτ
Dw Submerged depth of water in the inner of the pipe (m)
Do Outer pipe diameter (m)
Di Inner pipe diameter (m)
f0c Compressive strength of concrete (kN/m2)
fy Steel yield strength (kN/m2)
H Infill height placed upon the top of the pipe (m)
IM Impact factor
k Ratio of active unit pressure to vertical unit pressure
L Relative sample weight loss computed from data (%)
Final sample length side size in each perpendicular direction (cm)
Initial sample length side size in each perpendicular direction (cm)
M n Nominal bending capacity (kN−m)
pf Probability of failure
P Total live load applied at the surface (kN)
r Thickness loss versus sulfur availability rate (mm−cm2/mgS)
s(t) Compressive strength (M P a) measured in each exposed sample at time t si Initial strength (M P a) measured in the control sample at time t= 0.
Sa(τ) Sulfur availability (mgS/cm2) at timeτ
Salm =Limit (threshold) value ofSafrom which biodeterioration effects are evident (mg/cm2 )
t Real time measured during the experiment (days)
u Coefficient of friction between fill material and sides of trench
V o Initial volume of a sample computed from data (cc)
w(t) Dry weight (mg) measured at time t
wi Initial dry weight (mg) measured at time t= 0.
W f Measured final dry weight of a sample (g)
W o Measured initial dry weight of a sample (g)
W L Wheel load average pressure intensity (kN/m2)
W F Hydrostatic pressure at depth z(m) (kN/m2)
W P Pipe weight of a unit length arc (kN/m2)
W S Backfill pressure at the top of the pipe (kN/m2)
XR System resistance (i.e. bending moment capacity)
XS Effect of loads demanding the system (i.e. demanded bending moment)
α Bedding angle related to the soil reaction under the pipe ∆φ(t) Porosity variation
∆s(t) Compressive strength variation (%) ∆t(τ) Thickness loss (mm) at timeτ
∆w(t) Weight variation (%) ∆x, ∆y,
Thickness loss in each perpendicular directionx, y, z of a sample
φ(t) Porosity (%) measured in each sample at time t
φ(i) Initial porosity (%) measured in control sample at timet= 0
γ Backfill unit weight (kN/m3)
ρ Reinforcement steel ratio
σφ(Sa(ρ)) Standard deviation of porosity variation estimated using the model at time τ (%)
σs(Sa(ρ)) Standard deviation of strength variation estimated using the model at time τ (%)
σw(Sa(ρ)) Standard deviation of weight variation estimated using the model at time τ (%)
List of Figures
1.1 Examples of concrete biodeterioration (from http://www.engr.psu.edu) a) Exposed corroded reinforcement bars. b) Deteriorated concrete in sewer . . . 2 3.1 General experimental protocol . . . 20 3.2 Culture grown in tubes and plates: H. neapolitanus (left) andA.
thioox-idans (right) . . . 21 3.3 Orion 4Star pH meter and spectrophotometer Genesys 10UV (Thermor ) 22 3.4 100X photograph ofHallothiobacillus neapolitanus culture . . . 23 3.5 SEM image of initial inoculation withA. thiooxidans . . . 24 3.6 Casting and curing of samples . . . 28 3.7 Cubic 50mm×50mm×50mm samples made of ordinary mortar (OM mix) 29 3.8 Non-carbonated (left) and carbonated samples (right) before exposure.
In this picture, non-carbonated have the half of the size of carbonated samples . . . 32 3.9 Apparatus for samples exposure . . . 34 3.10 Portable Gas Analyzer BioGas CDM (LANDTECr) and RKI GX2009
(RKI Instruments r) . . . 35 3.11 Hydrogen sulfide concentration observed in one container forH2Speaks
up to 131 ppmv: a) total time window (heavy line shows the continuous equivalent concentration), b) example of applications during 5 consecu-tive days . . . 36 3.12 Hydrogen sulfide concentration observed in one container forH2Speaks
up to 222 ppmv: a) total time window (heavy line shows the continuous equivalent concentration), b) example of applications during 5 consecu-tive days . . . 37 3.13 Applied sulfur to exposed samples (sulfur availability) forH2Speaks up
to 131 ppmv. Coeficient of variation varies between 0.5 and 1.8% making the error bars invisible. . . 38 3.14 Applied sulfur to exposed samples (sulfur availability) forH2Speaks up
to 222 ppmv. Coeficient of variation varies between 0.7 and 2.6% making the error bars invisible. . . 39 3.15 Alicona Infinite Focus optical device r . . . 43
3.17 Typical scenario to take frames for volume determination from video technics . . . 48 4.1 Stage of biotic samples inoculated in non aseptic conditions grown in SM
after exposure: a) dried at 0 days, b) dried at 19 days, c) humid at 33 days, e) dried at 35 days, f) humid at 67 days, g) dried at 82 days, h) humid at 129 days . . . 54 4.2 Stage of H2S-only control samples after 153 days of exposure
manipu-lated in non aseptic conditions . . . 55 4.3 Surface of samples inoculated in non aseptic conditions in SM on days 0
and 48 of exposure (20X photograph) . . . 55 4.4 Surface of samples inoculated in non aseptic conditions grown in SM
after 62 days of exposure (20X photograph) . . . 56 4.5 Exposed samples inoculated in aseptic conditions: 1) H. n., 2) A.t.,
3a) H.n.+A.t., 3b) H.n.+A.t.+Triclosan, 4) H2S, 5) Control, 6) Non-carbonated . . . 57 4.6 Comparison at the end of the experiment. Left: Samples inoculated in
aseptic conditions (300 days); Right: Samples inoculated in non aseptic conditions (153 days) . . . 58 4.7 Antimicrobial effect of Triclosan in samples inoculated in aseptic
condi-tions after 150 days of exposure. Left: With no addicondi-tions; Right: Added with Triclosan . . . 58 4.8 Tridimensional images obtained using the Alicona Infinite Focusr . . . 59 4.9 Scaled picture (X100) obtained using the Alicona Infinite Focusr . . . 60 4.10 Typical parameters computed using the Alicona Infinite Focusr . . . . 61 4.11 Typical curves generated by the Alicona Infinite Focus r . . . 62 4.12 Superficial porosity evolution. COV: H.n. 3.5 to 4.2%, A.t. 11 to 15%,
Cons. 7.5 to 9.1%,H2S 8.6 to 12.1%, Control 8.1 to 9.8% . . . 64 4.13 Superficial irregularity evolution. COV: H.n. 12.1 to 16.9%, A.t. 15.4
to 22.0%, Cons. 11.3 to 15.1%, H2S 12.7 to 19.8%, Control 13.9 to 24.7%. 65 4.14 XRD analysis of biodeteriorated samples . . . 66 4.15 H.n. intensity toH2S intensity ratio . . . 68 4.16 A.t. intensity toH2S intensity ratio . . . 69 4.17 H.n.+A.t. intensity toH2S intensity ratio . . . 70 4.18 Reconstructed volume using video technics . . . 71 5.1 Humidity of exposed samples inoculated in non aseptic conditions. Error
bars show minimum and maximum values. . . 75 5.2 Weight loss of samples inoculated in non aseptic conditions using
stan-dard media . . . 77 5.3 Weight loss of samples inoculated in non aseptic conditions using salty
5.4 Average weight loss of samples inoculated in aseptic conditions . . . 80 5.5 Comparison between proposed curves and measured data for weight
changes in carbonated samples dried at 110oC- H.Neapolitanus . . . 81 5.6 Comparison between proposed curves and measured data for weight
changes in carbonated samples dried at 110oC -A.Thiooxidans . . . 82 5.7 Comparison between proposed curves and measured data for weight
changes in carbonated samples dried at 110oC - Consortium . . . 83 5.8 Comparison between proposed curves and measured data for weight
changes in carbonated samples dried at 110oC -H2S . . . 84 5.9 Comparison between proposed curves and measured data for weight
changes in carbonated samples dried at 110oC - Control . . . 85 5.10 Relationship between weight changes and sulfur availability . . . 86 5.11 Verification of purity of strains by stamping one face of exposed samples
upon Agar . . . 88 5.12 Total (open) porosity variation during exposure (inoculated in non
asep-tic conditions) . . . 91 5.13 Average mercury intrusion of samples Hn during exposure inoculated in
non aseptic conditions. . . 92 5.14 Average mercury intrusion of samples At during exposure inoculated in
non aseptic conditions. . . 93 5.15 Average mercury intrusion of samples nt during exposure inoculated in
non aseptic conditions. . . 94 5.16 Average mercury intrusion of control samples in case of non aseptic
con-ditions. . . 95 5.17 Average mercury intrusion ofH2Ssamples (case of non aseptic conditions). 96 5.18 Average mercury intrusion with respect to control (case of non aseptic
conditions). . . 97 5.19 Volume variation in pores smaller than 10 nm (case of non aseptic
con-ditions) . . . 98 5.20 Volume variation in pores between 10 and 5000 nm (case of non aseptic
conditions) . . . 99 5.21 Volume variation in pores larger than 5000 nm (case of non aseptic
con-ditions) . . . 100 5.22 Average mercury intrusion of pyritic samples at the experiment initiation.101 5.23 Porosity of samples inoculated in aseptic conditions . . . 103 5.24 Gap between mean and extreme values for H.n. samples . . . 104 5.25 Gap between mean and extreme values for A.t. samples . . . 105 5.26 Gap between mean and extreme values for H.n.+A.t. samples . . . 106 5.27 Gap between mean and extreme values for H2S samples . . . 107 5.28 Cumulative mercury intrusion (average data) versus pore size in
carbon-ated samples dried at 110oC inoculated in aseptic conditions. . . 109
5.29 Comparison between proposed curves and measured data for porosity changes in carbonated samples dried at 110oC -H.Neapolitanus . . . 110
5.31 Comparison between proposed curves and measured data for porosity changes in carbonated samples dried at 110oC - Consortium . . . 112
5.32 Comparison between proposed curves and measured data for porosity changes in carbonated samples dried at 110oC -H2S . . . 113 5.33 Comparison between proposed curves and measured data for porosity
changes in carbonated samples dried at 110oC - Control . . . 114 5.34 Typical compressive breaking of exposed samples . . . 117 5.35 Deteriorated strength-tested sample after 84 days of exposure . . . 118 5.36 Strength variation during exposure of samples inoculated with SM in
non aseptic conditions. . . 119 5.37 Strength variation after exposition of samples inoculated with MM using
non aseptic conditions . . . 120 5.38 Strength variation trend versus sulfur availability trend for samples
in-oculated in aseptic conditions . . . 122 5.39 Strength variation of samples inoculated in aseptic conditions . . . 123 5.40 Comparison between proposed curves and measured data for strength
changes in carbonated samples dried at 110oC inoculated in aseptic con-ditions - H.Neapolitanus . . . 125 5.41 Comparison between proposed curves and measured data for strength
changes in carbonated samples dried at 110oC inoculated in aseptic con-ditions - A.Thiooxidans . . . 126 5.42 Comparison between proposed curves and measured data for strength
changes in carbonated samples dried at 110oC inoculated in aseptic con-ditions - Consortium . . . 127 5.43 Comparison between proposed curves and measured data for strength
changes in carbonated samples dried at 110oC using aseptic conditions - H2S . . . 128 5.44 Comparison between proposed curves and measured data for strength
changes in carbonated samples dried at 110oC using aseptic conditions - Control . . . 129 5.45 Strength and porosity variation in samples inoculated in non aseptic
conditions. Each pair of data (porosity, strength) is measured at the same sampling time . . . 131 5.46 Strength losses associated to porosity and weight changes in
biodeteri-orated samples previously carbonated and dried at 110oC inoculated in aseptic conditions. Each pair of data (porosity increase, strength loss) or (weight loss, strength loss) is computed at the same sampling time . 133 5.47 Compressive strength to total porosity relations associated to
biodeteri-oration in samples carbonated and dried at 110oC inoculated in aseptic
6.1 Installation and loading conditions for pipes set into excavated soils (adapted from ) . . . 142 6.2 Typical loads demanding a sewer pipe. Bedding angle α value depends
on the bedding material quality  . . . 143 6.3 Spread load area configurations used in the evaluation of traffic loads
(adapted from ) . . . 145 6.4 Analysis sections (crown and waterline) for structural design of RC
sew-ers pipes . . . 146 6.5 Bilinear idealization of capacity loss during biodeterioration . . . 147 6.6 Typical breakings related to structural collapse in sewers  . . . 149 6.7 Theoretical relationship between initial and final volume of a
biodeteri-orated sample . . . 150 6.8 Average thickness loss produced by biodeterioration computed and fit
from data. One Standard Deviation (S.D.) bounds are shown. . . 151 6.9 Model used for validation (SAP2000) . . . 154 6.10 Model used for MATLABrcode design. Up: Validation using SAP2000r;
Down: Crown at point 10, waterline at points 4 and 16 . . . 154 6.11 Example of typical steel reinforcement. No detailing steel reinforcement
is shown . . . 159 6.12 Methodology for proposal application . . . 160
List of Tables
2.1 Cost arisen from sewers systems failure  . . . 8 3.1 Description of mortar samples used in the experiment development . . . 19 3.2 Description of medium used in cultures development (culture media) . . 22 3.3 Exposure conditions of OM samples inoculated in non aseptic conditions 25 3.4 Exposure environments of OM samples inoculated in aseptic conditions 25 3.5 Contents of containers for biodeterioration test of pyritic mortar . . . . 26 3.6 Exposure environments of TM samples inoculated with Consortia (Cons.). 26 3.7 Mixes for pyritic-mortar casting . . . 30 5.1 Some exposed surface/volume ratios (ESRV) used in previous
biodeteri-oration studies . . . 76 5.2 Average weight variations measured in pyritic samples during 153 days . 79 5.3 Equations of curves fittings for properties variation whenSa(t)≥0.006mg/cm2 87 5.4 Total porosity variation in biodeteriorated samples inoculated in non
aseptic conditions . . . 90 5.5 Initial and final porosities in pore ranges (from raw data, aseptic
condi-tions) . . . 115 5.6 Initial measured compressive strength of pyritic mortar samples . . . 121 5.7 Equations for relationships of changes in mechanical properties of
biode-teriorated samples inoculated in aseptic conditions . . . 134 5.8 Equations for relationships between Compressive Strength (s) in MPa
and Total Porosity (φ) in % of biodeteriorated samples inoculated in aseptic conditions . . . 136 6.1 Real H2S concentrations (ppmv) reported in literature. All the
infor-mation has been taken from the work of Wells and Melchers (2015)  155 6.2 Suggested values for Monte Carlo simulation . . . 158 6.3 Design Service Life (DSL) for given total concrete covers . . . 161 6.4 Recommended minimum concrete cover for DSL=15,20 and 25 years
Description of the problem
Reinforced concrete (RC) is the hybrid material most used in construction worldwide and its importance in modern engineering is paramount. Reinforced concrete is a non-homogeneous material made of cement, aggregates (sand and gravel) and water, into which steel bars are embedded. Cement (Portland type) is mainly composed of dicalcium silicate (2CaOSi2) (C2S), tricalcium silicate (3CaOSi2) (C3S), trical-cium aluminate (3CaOAl2O2) (C3A), tetracalcium aluminoferrite (4CaOAl2O3F e2O3) (C4AF), calcium sulfate or gypsum (CaSO42H2O), free lime and other compounds in small amounts. After hydration of the cement, calcium silicate hydrate C-S-H (3CaO2SiO24H2O) and Portlandite (Ca(OH)2) are the most abundant and impor-tant products . The presence of Portlandite in hardened cement paste can facilitate concrete deterioration as described in the following paragraphs.
RC constructions are subjected to different anthropic and natural hazards that cause the material to deteriorate. Concrete deterioration in RC structures can come in different forms. Sudden events (e.g. earthquakes, cyclones) or sustained demands caused by operation or environmental factors can lead to loss of structures’ capacity. Large economic losses are usually associated with maintenance and recovery of deterio-rated structures arising from physically, chemically and biologically adverse conditions.
As a result, RC structures’ lifetimes can be severally reduced, bringing discomfort, un-expected costs, health problems, environmental detriment and low levels of service to a society.
The biological deterioration (biodeterioration) caused by microorganisms is a mech-anism that has not been sufficiently studied yet. Nevertheless, the so-called microbial induced concrete corrosion (MICC) has become an important engineering issue in the last years. Understanding biodeterioration requires the consideration of both physical and chemical mechanisms by which microorganisms attack the material. In concrete structures, biodeterioration increases porosity and contributes to crack growth in the concrete matrix . Proliferation of cracks and porosity augmentation in concrete that covers steel bars increases the rebars’ exposure to the environment (e.g., chlorides, bac-terial activity). In particular, changes in alkalinity from biological activity contribute to the depassivation of the reinforced steel surface, accelerating steel corrosion . As a result, biodeterioration becomes a facilitator of failures in in RC structures (Figure 1.1).
Figure 1.1: Examples of concrete biodeterioration (from http://www.engr.psu.edu) a) Exposed corroded reinforcement bars. b) Deteriorated concrete in sewer
Background of biodeterioration
Biodeterioration is defined as a reduction in material quality produced by vital activities of microorganisms . For a better understanding of biodeterioration, it is helpful
1.3 Research objectives
to examine bioreceptivity, which is related to the intrinsic capability of a material to allow its colonization as well as the development living organisms    . The bioreceptivity of concrete in indoor and outdoor environments can vary from inappreciable to very intense, influencing the biodeterioration start time .
Biodeterioration can be classified as: a) physical or mechanical; b) aesthetic; or c) chemical . Physical or mechanical biodeterioration occurs when living organisms pro-duce material breaking. In aesthetic biodeterioration organisms such as mold, mycelium and microalgae lead to surfaces fouling or soiling . Finally chemical biode-terioration can come through assimilatory or dissimilatory paths. In assimilatory path organisms feed from material, while in dissimilatory path organisms excrete harmful products that damage it.
Between the previously described biodeterioration processes, chemical biodeterio-ration is usually the most aggressive. It is commonly produced from bacterial growth and requires humidity, cycles of humidification and drying, appropriate acidity and environmental nutrients to be viable. Bacteria, fungi, algae and lichens are the main organisms involved in concrete biodeterioration . A comprehensive description of the processes and microorganisms related to concrete biodeterioration is presented in chapter 2.
The contribution of this study is the assessment of the physical (porosity and weight) and mechanical (i.e., compressive strength) consequences of biodegradation in mortar samples. The results would contribute to a better description of concrete biogenic corrosion processes, and consequently, to provide specific quantitative knowledge on concrete biodeterioration effects. This information is needed to improve the assessment of biodeterioration effects on concrete durability over time.
The specific objectives of this work are summarized as follows:
the physical properties (i.e., porosity and weight) of high surface/volume-ratio mortar samples.
To determine how biodeterioration produced by sulfur oxidizing bacteria affects the mechanical properties (i.e., compressive strength) of high surface/volume-ratio mortar samples.
To compare the effects produced by biogenic and chemical attack upon high surface/volume-ratio mortar samples.
To evaluate the influence of sulfur availability on the biodeterioration produced by sulfur oxidizing bacteria upon high surface/volume-ratio mortar samples.
To estimate the probability of failure of sewer pipes considering experimental results, and suggest the use of sacrificial layers in sewers pipes for guaranteeing given design service life values.
This document is divided into six chapters. Chapter 1 presents the background and objectives of the thesis.
Chapter 2 describes the fundamentals of the concrete biodeterioration processes. In-fluence of biodeterioration in costs related to maintenance needs or reduction of service life of infrastructure systems is discussed. Also a description of the biodeterioration of sewers is presented. Finally, a summary of the more studied bacteria related to concrete biodeterioration and their effect upon the concrete health is presented.
Chapter 3 summarizes the applied experimental design. It explains the way in which the mortar samples were manufactured, inoculated and exposed to different environments. A description of the most important tests and the data to be collected is also presented. Data coming from qualitative description and variations in geometry, weight, porosity and strength of the samples are the most important outputs of the experimental work.
1.4 Thesis organization
Chapter 4 presents the results and discussion of the preparations and general tests related to the experimental work. Descriptions of the bacterial growth and the sulfur availability achieved during the experiment are presented. Also results from chemical, topographic and volumetric tests such are summarized and interpreted.
Chapter 5 presents the results and discussion related to the physical and mechanical tests. Observed weight, porosity and compressive strength variations in mortar samples are described and analyzed. Besides, the strength to porosity relation is found and interpreted.
In chapter 6, a preliminary approximation to consider the effect of biodeterioration in practical applications is described. Firstly, the current practice in structural design of sewers is summarized. Secondly, the effects of the biodeterioration upon strength and inner forces redistribution are illustrated by an example. Thirdly, the probability of failure for different exposure and manufacturing conditions is computed. Finally, a proposal for including the effects of biodeterioration in the structural design of sewers is presented.
In chapter 7 the conclusions and recommendations of the thesis are presented. Also some ideas and suggestion for future work are given.
As explained in chapter 1, chemical biodeterioration produced by biongenic activity affects the concrete. It is necessary to understand how such processes occur. To achieve that, in this chapter a comprehensive description of the biodeterioration dynamics is presented. Then, in the following chapter the experimental development used in this study will be described. The objectives of this chapter are:
To discuss critically the importance of the adverse effects of biodeterioration upon infrastructure systems, such as capacity and durability decrements, according to the existing literature and reports of previous studies.
To describe how the chemical and biological processes affect the concrete sewers, underlining those related to the acidification of concrete surfaces.
To describe bacteria that produce the most adverse effects related to biodeteri-oration of RC structures. This objective refers mainly sulfur oxidizing microor-ganisms
Importance of the biodeterioration effects upon
Biodeterioration is usually overlooked because its kinematics is very slow and there-fore, it remains undetected or neglected during the structural lifetime. Furthermore, although biodeterioration itself is rarely a direct cause of failure, it may play an impor-tant role in reinforced concrete degradation by accelerating other damaging processes such as chloride ingress (e.g., in marine environments or in structures subjected to de-icing salt) and carbonation. These processes lead to corrosion propagation and loss of structural capacity .
The life-cycle analysis and modeling of infrastructure requires the understanding of concrete performance over time, which highly depends on the characterization of material degradation . Although phenomena such as aging, fatigue and cor-rosion are known to be important agents for concrete degradation, it has been noted that in aggressive environments, the action of living organisms also affects critical in-frastructure. These problems have been reported in, for example, oil pipelines , underground structures, sewage systems, and offshore structures . Biodete-rioration affects mainly concrete durability increasing maintenance costs , and reducing the capacity of structural members in the long term. Table 2.1 presents a summary of real costs associated to sewers failure.
Table 2.1: Cost arisen from sewers systems failure 
Asset description Cost US$ billion/yr Sewers replacement/Los Angeles, USA 468
Infrastructure repair and maintenance/United Kingdom 2,300 Sewers repair and maintenance/Belgium 6
2.3 Consequences of biodeterioration
Consequences of biodeterioration
2.3.1 Effects on concrete properties
Several studies have focused on the weight loss as an indicator of biodeterioration activity . They report a wide range of weight loss observations (even for similar environmental conditions) ranging from negligible weight loss after 126 days of exposure  to total weight loss (100%) after 350 days . The heterogeneity of the cementitious mortars and concrete, the variability of the environmental conditions, and the interactions and dynamics of the microorganisms involved in sulfur oxidation are only some of the aspects adding complexity to the description and quantification of the biodeterioration process .
Bielefeldt et al. measured a weight loss of 0.45% in samples cut from concrete pipes after 83 days of exposure toThiobacilli sp. consortia and A. cryptum in a 300-600 ppmvH2Satmosphere. Microbiological tests conducted by Monteny et al. showed that acidophilic microorganisms activity produced greater biodeterioration (weight loss up to 8%) than exclusive chemical effect (immersion and rotation in sulfuric acid) . Parker and Prisk reported a weight loss of up to 12% after 90 days of exposure to sulfuric acid at pH=1.5 in plain concrete . Starkey investigated the effect ofThiobacilli sp.
by exposing concrete samples to H2S, thiosulfate and methylmercaptan and found that bacterial growth only occurred in the first two. T. thiooxidans dominated the flora in the H2S-rich environment while H. neapolitanus showed remarkable growth when thiosulfate was used as the main nutrient. T. thiooxidans produced the most severe deterioration with a weight loss of up to 5.8% after nine months of exposure .
Vollertsen et al. reported that even H2S concentrations as low as 50-10 ppmv can produce deterioration in concrete sewers of up to several mm/year . Aviam et al. usedH. neapolitanus to degrade cement mortar samples and showed that a weight loss of up to 16% after 39 days of exposure is possible . Okabe et al. measured weight losses of up to 37% in concrete coupons exposed to a succession of SOB for one year
. Wells and Melchers reported that corrosion rates of old concrete were up to one order of magnitude greater (up to 7 mm/year) than those of new concrete . They measured in situ H2S concentrations of up to 680 ppmv , which could not necessarily be associated with the most severe corrosion compared to lower-H2S-concentration environments. Beeldens et al., using microscope techniques, observed adverse effects of chemical and biogenic acid corrosion in concrete samples when exposed up to 250 ppmvH2S .
In addition to weight loss, biodeterioration can also affect other physical and me-chanical properties of concrete. During concrete biodeterioration, a layer of high poros-ity is produced by biogenic attack. This high porosporos-ity layer leads to greater perme-ability and diffusion within the inner matrix of the material . On the other hand, compressive strength decreases for larger porosities in concrete and mortar spec-imens . Consequently, the compressive strength of concrete components is affected by biodeterioration and must therefore be modeled as a time-variant property throughout the structural lifetime . Although porosity and strength variations due to biodeterioration are paramount for structure condition assessment, to the authors’ knowledge, nowadays there are no studies that include these parameters.
The relationship between compressive strength and porosity of concrete has not been sufficiently studied . Some studies have investigated the effects of normal and acidic conditions on these two parameters, leading to models in which strength decreases while porosity increases . For example, Kumar and Bhattacharjee exposed concrete specimens made of quartzite aggregates to atmospheric conditions and chemical acidic water reporting porosity values from 9.26% to 13.53% with no apparent preponderance of acidic conditions . Sol´ıs-Carca˜no and Moreno described porosity variations from 18.8% to 25.2% for water/cement ratios from 0.45 to 0.80 in a wide range of types of aggregates . Ba et al. concluded that coarse pores have the most important influence on compressive strength . Hincapi´e and Montoya found that dry concretes show major porosity that normal concretes but this condition does not affect the strength . On the other hand, Bastidas et al. explained that,
2.4 Biodeterioration in sewers
once the steel corrosion process has been initiated in RC structures, low-density steel corrosion products fill the porous structure surrounding steel reinforcement and produce a volume increase that leads to cracking . However, there is no concluding evidence from previous research related to the effect of biogenic attack on porosity and strength, making this an important issue to investigate. In summary, a good understanding of the porous structure of concrete is undeniable important.
2.3.2 Effects on chloride ingress
Another important aspect related to concrete biodeterioration is the effect of chloride ingress in offshore and inshore reinforced concrete structures like bridges . Is is possible to find some sulfur oxidizing bacteria (SOB) belonging to theThiobacillispecies in the sea resulting in a possible path to biodeterioration by bacterial attack in chloride-rich environments . Nevertheless, in most cases salty environments can inhibit
Thiobacilli growth . Biodeterioration weakens the RC matrix favoring cracking and porosity increase which facilitate chloride ingress. Chloride ingress through cracks or capillary structures within the concrete matrix leads to steel corrosion in RC structures. Moreover, steel reinforcement can also be corroded when exposed to sulfur-containing gases or microbial activity in the surrounding concrete .
Several models have attempted to describe and forecast chloride diffusion in satu-rated and non-satusatu-rated concrete . There are also widely accepted tests to evaluate chloride diffusivity, like those stated in AASHTO T259 (ponding test) and ASTM C1202 (electrical conductance). This section is only intended to inform about the importance of the described topics and no work has been done related to this issue.
Biodeterioration in sewers
2.4.1 Chemical and biological deterioration in sewers
Hydrogen sulfide can be present in natural emissions, industrial waste, landfills, within sewers, and elsewhere. In concrete structures it can cause acidification directly from
chemical attack or indirectly from biological byproducts from microorganisms that use it as energy source. Nevertheless, sewer systems are known as one of the most prob-able and important biodeterioration targets. Permanent moisture, oxygen and water availability, formation of biofilms under anaerobic conditions, existence of partially oxi-dized sulfur compounds andH2S, and warm temperatures can usually be found within sewers. In these systems, due to anoxic conditions commonly found in sewage, sulfate in wastewater is used by sulfur reducing bacteria (SRB) as an electron acceptor and sulfide is produced. At low pH, hydrogen sulfide gas volatilizes and rises to the tops of sewer pipes where aerobic microbial communities grow in biofilms . Sulfur oxidizing bacteria (SOB) living in these biofilms use hydrogen sulfide or reduce sulfur compounds as electron donors and oxygen from air as an electron acceptor. The oxida-tion process generates sulfate or sulfuric acid . The main consequence of sulfuric acid attack is the modification of the C-S-H structure of concrete that results from the reaction of sulfate ions with the cement hydration products. This process results in the formation of gypsum and ettringite, leading to the destruction of the hydration products that constitute the binder of concrete. The formation of ettringite may lead to increased tensile stress within the concrete matrix, resulting in cracking .
H2S present in sewers is removed chemically by walls’ sorption and biologically by bacterial metabolism in a process in which H2S sorption to concrete surfaces is quite similar to H2S biological uptake . Cell adhesion and sulfuric acid attack are interfacial phenomena that depend on the surface area/surface roughness ratio . The microbial succession is a surface phenomenon in which the Acidophilic Sulfur Oxidizing Microorganisms (ASOM) move into the corroding concrete while it becomes deeper but Neutrophilic Sulfur Oxidizing Microorganisms (NSOM) do not . It has been observed that typical microorganisms in sewers are able to survive starvation up to for six months, recovering up to 80% of their initial growth rate when subjected to
2.4 Biodeterioration in sewers
2.4.2 Sewer environment conditioning for biodeterioration
The ecology of the sulfur oxidizing microbial communities is highly dependent on the pH of the concrete matrix  . After casting, the pH of concrete is higher than 12 (usually in the order of 13.5), which inhibits sulfur-oxidizing bacteria development. This alkalinity is produced mainly by formation of calcium hydroxide,Ca(OH)2, dur-ing cement hydration. In sewer pipes, however, carbonation and exposure to hydrogen sulfide reduces concrete pH to a point at which neutrophilic microorganisms can grow. Among these, SOB grow and produce sulfuric acid (H2SO4), which also lowers the pH even further to a point at which acidophiles thrive. These new conditions trigger mi-crobial growth with its correspondent metabolic byproducts. The so produced sulfuric acid reacts with calcium-hydroxide forming gypsum (CaSO42H2O). Gypsum reacts with tricalcium aluminate, leading to the formation of secondary ettringite (calcium trisulfoaluminate hydrate, 3CaOAl2O33CaSO432H2O). Secondary ettringite causes swelling inside the concrete matrix, breaking its inner structure. .
When the typical pH of sewage environments has dropped to values lower than 6 or 7, H2S becomes the dominant compound, which, in the presence of oxygen and sulfides, promotes the formation of partially oxidized sulfur like thiosulfate, elemental sulfur and polysulfate. These reactions, the turbulence of flow, the diameter of pipe and the depth of flow facilitate the augmentation of H2S ingress into the condensed layer attached to the pipe walls. Then, because of the presence of CO2,H2S, oxygen, moisture and nutrients, Thiobacilli sp. can obtain energy, oxidizing sulfur to sulfuric acid (H2SO4) and growing in the new environment . In general, it has been found that pH variations in concrete specimens subjected to biogenic attack are related to biodeterioration severity .
2.4.3 Bacteria species related to concrete biodeterioration
Biodeterioration from bacteria has been found to produce damage to aerial and buried RC structures. Sulfur-oxidizing bacteria and nitrifying bacteria can generate biogenic products that damage the concrete. T. thioparus (pH 4.5-10), T. novellus (pH 5-9.2),
H. neapolitanus(pH 4-9),T. intermedius (Thiomonas intermedia, pH 1.7-9), Leptospir-ilium ferrooxidans (pH 1.3-4.0),T. ferrooxidans (pH 1.5-3.3),A. cryptum (pH 0.1-5.2),
A. thiooxidans (pH 0.5-4, formerlyT. thiooxidans),Thiothrix sp.,T. plumbophilus, and
A. acidophilumn are found in sewer environments . Acidithiobacil-lales (which include A. thiooxidans) can represent only 4% of the total community living in sewers . However, within this order, Acidithiobacillus thiooxidans (for-merlyThiobacillus thiooxidans) has been found to be the most aggressive to concrete . Other microorganisms such as thefungus Fusariumhave been found to be harmful to concrete . Nevertheless, Acidophilic Sulfur Oxidizing Microorganisms (ASOM) have been found to be more aggressive than Neutrophilic Sulfur Oxidizing Microorganisms (NSOM) and other bacteria an fungi.
In this study, one neutrophilic and one acidophilic bacterium have been selected for the experiment: Hallothiobacillus neapolitanus and Acidithiobacillus thiooxidans. The reason for this selection is that H. neapolitanus can be found on concrete at the beginning of the biocolonization when the pH is still high while A. thiooxidans thrives when pH is low. The optimum pH for the development of such bacteria varies about 6.7 and 3.0 for H. neapolitanus and A. thiooxidans, respectively .
Acidithiobacillus thiooxidans can be found in soils but are unable to survive after 24 hours of drying. However, it has been observed that these bacteria are able to develop after long periods of laboratory incubation .
In summary, Acidithiobacillus thiooxidans is an acidophilic and autotrophic bac-terium capable of oxidizing sulfur compounds and obtaining its carbon from atmo-spheric CO2. It is an aerobic obligately acidophilic Gram-negative bacterium that is motile by a polar flagellum and uses elemental sulfur, thiosulfate or tetrathionate. This bacterium, in the presence of oxygen, can convert hydrogen sulfide (H2S) to sulfuric acid (H2SO4) . A culture ofThiobacillus thiooxidans is not a homogenous commu-nity, but rather a set of organisms at different stages of development .
Hallothiobacillus neapolitanus, probably first isolated from sea water in Naples in 1902, is a halophile obligately chemolithoautotrophic Gram-negative bacterium that
2.5 Summary and conclusions
obtains its energy from reduced inorganic sulfur compounds, among which thiosulfate is the best suited for optimal growth. This species was initially classified asThiobacillus X and has been isolated from seawater and compost .
Summary and conclusions
The following conclusions respond to the objectives written at the beginning of this chapter.
The biogenic and chemical deterioration can potentiate the physical damage due to the chemical reactions leading to the structural breaking of the concrete ma-trix. It has been observed that biogenic deterioration (biodeterioration) is usually faster and more catastrophic than pure chemical or physical deterioration.
It has been found thatAcidithiobacillus thiooxidansare the most harmful bacteria related to the concrete biodeteriortaion in sewers. Other microorganisms like the fungus Fussarium and the neutrophilic bacteriaHallothiobacillus neapolitanus
have been found to be less aggressive but important to the sewer biodeterioration processes.
Weight loss, porosity augmentation, and strength decrease are the most adverse changes resulting from concrete biodeterioration. Cracking and consequent per-meability increase related to the described effects facilitate the chloride ingress and steel rebar corrosion shortening the structural durability.
Several reports related to the concrete biodeterioration based on weight loss measure-ments were cited in the previous chapter. No information related to the porosity and strength changes using the same samples is found in the literature. For this reason, in this study weight, porosity, and compressive strength variations produced by biodeteri-oration in mortar samples were measured. Such changes were measured using samples which have a high exposed surface in a non-aqueous environment.
This chapter presents the design of the experiment and its objectives are:
To develop a methodology for measuring and interpreting the physical and me-chanical changes produced by biodeterioration in mortar samples within a con-trolled environment.
To design the experimental setup for manufacturing, conditioning, exposing, and measuring the mortar samples behavior when deteriorated by biogenic attack.
To interrelate the physical, chemical and biological processes using the same sam-ples and environmental conditions to facilitate a comprehensive interpretation of the results.
Basic principles of the experiment
As explained in chapter 2, most previous studies have focused their experiments on weight loss measurements. Samples used in those works have usually been cut and brushed to determine such measurements. In this study, not only weight losses were determined but strength and porosity were measured using scaled tests for the first one and mercury intrusion porosimetry technics for the second one. In addition, samples were not manipulated excesively. No brushes or cutting tools were used to modify the final condition of samples. Also, in this study samples have a high exposed surface to volume ratio (ESV). This feature and the low saturation degree of the surfaces (non-aqueous) probably impose to this experiment a more severe condition than previous studies.
Figure 3.1 presents a graphical summary of the experimental protocol. Four oper-ational fringes have been defined for this study:
First fringe (green) describes the biological processes in which the bacterial strains are resuscitated, cultured and precipitated. All these processes were made fol-lowing the recommendations of the supplier of microorganisms. At the end of this fringe inoculum to be applied to samples was ready to use. This part of the protocol is explained in section 3.3.
Second fringe (yellow) refers to the production of samples hospitable to the inocu-lum. Manufacturing, carbonation and sterilization of mortar samples are included in this part of the protocol. Also two common activities (samples inoculation and samples exposure) are considered in this fringe. Samples inoculation requires to apply the result of the first fringe upon the solid samples prepared as explained. Then, inoculated samples are exposed to the environment generated in the third fringe. In section 3.4. this part of the protocol is explained.
Third fringe (violet) shows the procedures followed to manufacture containers and calibrate and produce the gaseous environment required at the inner of them. More details of this part of the protocol are described in section 3.5.
3.2 Basic principles of the experiment
Fourth fringe (white) contains the processes related to the mechanical and phys-ical tests to be applied to the samples.
In this study three classes of samples were prepared:
OM: Ordinary mortar samples whose characteristics are described in table 3.1 and section 3.4.1.
PM: Pyritic mortar samples whose characteristics are described in table 3.1 and section 3.4.2.
TM: Mortar samples added with Triclosan (TM) whose characteristics are de-scribed in table 3.1 and section 3.4.3.
Table 3.1: Description of mortar samples used in the experiment development Class Name Raw material and additions Qty
OM Ordinary mortar samples Portland cement, river sand, water 1.200 PM Pyritic mortar samples OM, Fe, S orF eS2 1.500
Figure 3.1: General experimental protocol
3.3 Culture growth and inoculation of mortar samples
Culture growth and inoculation of mortar samples
Hallothiobacillus neapolitanus NCIMB 8454 andAcidithiobacillus thiooxidans NCIMB 9112 (ATCC8085) were purchased from American Type Culture Collection (ATCC) (Virginia, USA). Pure cultures were grown in DSMZ (Deutsche Sammlung von Mikroor-ganismen und Zellkulturen) 68Thiobacillus neapolitanus agar/liquid medium or DSMZ 35 Thiobacillus thiooxidans agar/liquid medium, as recommended by supplier. Figure 3.2.
Figure 3.2: Culture grown in tubes and plates: H. neapolitanus (left) andA. thiooxidans
In order to evaluate the effect of NSOM and ASOM on mortar biodeterioration, the prepared samples were subjected to different bacterial attack environments. NSOM
Hallothiobacillus neapolitanus (H.n.) and ASOM Acidithiobacillus thiooxidans (A.t.)
growth in six standard and four salty media was implemented. DSMZ 68 Thiobacillus neapolitanus liquid medium and DSMZ 35Thiobacillus thiooxidans liquid medium led to the best behavior of bacterial development in both standard (SM) and salty liquid (MM) (Table 3.2).
Figure 3.3: Orion 4Star pH meter and spectrophotometer Genesys 10UV (Thermor )
Prior to inoculating mortar samples, bacterial cells were grown in liquid media to an optical density (OD) 600 of 1.0. Figure 3.3. Cultures were centrifuged (4oC, 13000 rpm, 15 min) to separate cells from growth medium and were triple washed with mineral medium containing no source of sulfur. Washed cells suspended in mineral medium (without sulfur) were used to inoculate mortar samples. Oven-dried mortar samples were soaked in cell suspensions of A. thiooxidans, H. neapolitanus, or a consortium of both.
Table 3.2: Description of medium used in cultures development (culture media) Medium
Samples SM Standard liquid medium (DSMZ 68 or DSMZ 35) Hn,At,nt MM Seawater modified liquid medium (DSMZ 68 or DSMZ 35) Hns,Ats.nts
In order to have cultured bacteria available at any moment, the first incubated liquids were mantained, renovating them with fresh media approximately once a
fort-3.3 Culture growth and inoculation of mortar samples
night. Furthermore, pH variation was measured throughout the experimentation time to verify that the bacteria were actually growing. pH variation was measured using an Orion 4Star pH meter (Thermor) (Figure 3.3).
Fresh inoculated media were applied to the samples three times on days 0, 15 and 30 to guarantee an initial bacterial dynamic activity.
Acidithiobacillus thiooxidans showed a similar growth rate in both SM and MM me-dia, whileHallothiobacillus neapolitanus developed ten times faster in the salty medium than in the standard medium.
Figure 3.4: 100X photograph of Hallothiobacillus neapolitanus culture
In order to check the morphology of bacteria stuck on sample surfaces, microscope and SEM images were taken on day 15 of the experiment (Figure 3.4) and (Figure 3.5).
Figure 3.5: SEM image of initial inoculation withA. thiooxidans
3.3.1 Inoculation of OM samples in non aseptic conditions
Sterilized OM samples were submerged during 30 seconds into SM and MM media as described in Table 3.3. Then they were put into the apparatus described in section 3.6. In this case, no sterile conditions were guaranteed when manipulating the samples through the whole duration of the experiment. The term “non aseptic conditions”refers to the possible existence of many other microorganisms capable of surviving in the given experimental environment which could ingress to the containers while samples were extracted.
3.3 Culture growth and inoculation of mortar samples
3.3.2 Inoculation of OM samples in aseptic conditions
Sterilized OM samples were submerged during 30 seconds into SM media as described in Table 3.4. Then they were put into the apparatus described in section 3.6. In this case, sterile conditions were guaranteed when manipulating these samples through the whole duration of the experiment to guarantee the purity of strains within the containers.
Table 3.3: Exposure conditions of OM samples inoculated in non aseptic conditions Sample Superficial treatment (inoculation) Environment
Hn H.neapolitanus standard medium (SM) ≤222 ppmvH2S, 0.3±0.1%CO2
At A. thiooxidans standard medium (SM) ≤222 ppmvH2S,0.3±0.1%CO2
nt Consortium (H.n+A.t.) standard medium (SM) ≤222 ppmvH2S, 0.3±0.1%CO2
ctrl Abiotic control Ordinary humid atmosphere H2S Chemical control ≤222ppmv H2S
Hns H.neapolitanus seawater medium (MM) ≤222 ppmvH2S, 0.3±0.1%CO2
Ats A. thiooxidans seawater medium (MM) ≤222 ppmvH2S, 0.3±0.1%CO2
nts Consortium (H.n+A.t.) seawater medium (MM) ≤222 ppmvH2S, 0.3±0.1%CO2
Table 3.4: Exposure environments of OM samples inoculated in aseptic conditions Sample Name Superficial treatment (inoculation) Feeding conditions
H.n. H. neapolitanus standard medium ≤131 ppmv H2S, 0.3±0.1% CO2
A.t. A. thiooxidans, standard medium ≤131 ppmv H2S, 0.3±0.1% CO2
Cons. Consortium, standard medium ≤131 ppmv H2S, 0.3±0.1% CO2
H2S Chemical exposure (abiotic) ≤131 ppmv H2S, 0.3±0.1% CO2
Ctrl. Control Ordinary humid atmosphere
3.3.3 Inoculation of PM samples in non aseptic conditions
Sterilized PM samples were submerged during 30 seconds into SM and MM media as described in Table 3.5. Then they were put into the apparatus described in section 3.6. No sterile conditions were guaranteed when manipulating these samples through the whole duration of the experiment. The term “non aseptic conditions”refers to the possible existence of many other microorganisms capable of surviving in the given experimental environment which could ingress to the containers while samples were extracted.
Table 3.5: Contents of containers for biodeterioration test of pyritic mortar
Sample Name Addition Bacteria and environment
HnF1 Fe: 0.47% H.neapolitanus, 30oC, 50±10% HR HnS1 S: 0.53% H.neapolitanus, 30oC, 50±10% HR HnFS1 FeS2: 1.00% H.neapolitanus, 30oC, 50±10% HR HnF5 Fe: 2.35% H.neapolitanus, 30oC, 50±10% HR HnS5 S: 2.65% H.neapolitanus, 30oC, 50±10% HR HnFS5 FeS2: 5.00% H.neapolitanus, 30oC, 50±10% HR AtF1 Fe: 0.47% A. thiooxidans, 30oC, 50±10% HR AtS1 S: 0.53% A. thiooxidans, 30oC, 50±10%HR
AtFS1 FeS2: 1.00% A. thiooxidans, 30oC, 50±10% HR AtF5 Fe: 2.35% A. thiooxidans, 30oC, 50±10% HR AtS5 S: 2.65% A. thiooxidans, 30oC,50±10% HR AtFS5 FeS2: 5.00% A. thiooxidans, 30oC, 50±10% HR F1 Fe: 0.47% Non-inoculated, 30oC, 50±10% HR
S1 S: 0.53% Non-inoculated, 30oC, 50±10% HR FS1 FeS2: 1.00% Non-inoculated, 30oC, 50±10% HR F5 Fe: 2.35% Non-inoculated, 30oC, 50±10% HR
S5 S: 2.65% Non-inoculated, 30oC, 50±10% HR FS5 FeS2: 5.00% Non-inoculated, 30oC, 50±10% HR Ctrl 0% Non-inoculated, 30oC, 50±10% HR
3.3.4 Inoculation of TM samples in aseptic conditions
Sterilized TM samples were submerged during 30 seconds into SM media as described in Table 3.6. Then they were put into the apparatus described in section 3.6. Ster-ile conditions were guaranteed when manipulating these samples through the whole duration of the experiment to guarantee the purity of strains within the containers.
Table 3.6: Exposure environments of TM samples inoculated with Consortia (Cons.).
Sample Name Aggregate replacement Environment
T1 0.25% Triclosan ≤131 ppmv H2S, 0.3±0.1% CO2 T2 0.50% Triclosan ≤131 ppmv H2S, 0.3±0.1% CO2 T3 1.00% Triclosan ≤131 ppmv H2S, 0.3±0.1% CO2 H2S Chemical exposure (abiotic) ≤131 ppmv H2S, 0.3±0.1% CO2 Ctrl. Control Ordinary humid atmosphere
3.4 Sample casting and curing
Sample casting and curing
The following three classes of samples were cast and exposed to different environments. Both classes were made using Type I Portland Cement (Cement).
Ordinary mortar samples (OM). These samples were made using Cement, River Sand and Water. They were inoculated and exposed to two different H2S-rich environments as explained later as shown in Table 3.3 and 3.4
Pyritic mortar samples (PM). These samples were made using Cement, River Sand mixed with variable proportions of F eS2, Fe, S, and water. They were inoculated and exposed partially submerged in water to ordinary environment as shown in table 3.5.
Mortar samples added with Triclosan (TM). These samples were made using Cement, River Sand and Water. Little amounts of Triclosan were added. They were inoculated in aseptic conditions using a consortia of two strains and exposed to two one H2S-rich environment as shown in table 3.6.
3.4.1 Ordinary mortar samples (OM)
Portland cement mortar 13mm×13mm×10 mm samples with water-to-cement ratios of 0.485 were cast into a plastic container without a mold release agent. Casting was made by compacting two successive layers with a plastic rammer after 30 seconds of vibration with a pneumatic motor table. ASTM C778-06 standard graded natural river sand and Portland cement type I were used. Commercial cement was used. No further chemical analysis was applied to the cement. Cement paste-sand mix was blended using a five-pound mixer (Hamilton Beach Commercial) with a cement-to-sand relationship of 1:2.75. Afterward, casting molds containing fresh samples were wrapped with stretch film and stored at 20oC for 24 hours. During 30 days demolded samples were twice a day water sprayed and kept in an airtight container for curing (90%±5 relative humidity (RH) measured at headspace). Cured samples were oven dried at 110oC for
Figure 3.6: Casting and curing of samples
24 hours and then subjected to an “ordinary atmospheric”period for another 60 days at 20±2oC and 60±10% RH (Figure 3.6). This two-month initial phase attempted to simulate the typical waiting period before new sewer pipes are put into service. RH and temperature measurements were taken using a digital thermo-hygrometer Thermor. During the curing and preparation period samples were not oven-dried. Oven-drying was carried out only prior to the weighing process and for sterilization.
A strength scaling process was carried out to extrapolate the results to 13mm×13mm
×10mm samples. In order to have a valid pattern to compare strength results obtained for samples, 50mm-side cubic samples were cast, cured and exposed under similar con-ditions to those of 13mm×13mm ×10mm samples (Figure 3.7). 50mm-side samples were made of ordinary Portland cement mortar using OM mix and following ASTM C109/C109M12. See section 3.8.3.
3.4.2 Pyritic mortar samples (PM)
This section describes the experimental conditions for high surface/volume-ratio pyritic mortar samples to bacterial attack in a moist environment at 30oC and with continuous availability of atmospheric oxygen.
Samples of 13mm×13mm×10mm made of Portland cement and pyritic aggregates mortar with a water-to-cement ratio of 0.485 were cast into a plastic container without
3.4 Sample casting and curing
Figure 3.7: Cubic 50mm×50mm×50mm samples made of ordinary mortar (OM mix)
a mold release agent. Casting was done by hand, compacting two successive layers with a plastic rammer after 30 seconds of vibration with a pneumatic motor table. ASTM C778-06 standard-graded natural river sand, pyrite, sulfur, iron, and Portland cement type I were used. Content of additions in percentage of weight of the aggregate are shown in Table 3.7. Pyrite and sulfur additions were sieved 50% below mesh size 16 and 50% below mesh size 50 (grain sizes smaller than 1.52 mm and 0.30 mm, respectively). Samples containing 0% additions were also cast to be exposed to ordinary atmospheric environment. Cement paste-aggregate mix was blended using a five-pound mixer (Hamilton Beach Commercial) with a cement-to-aggregate relationship of 1:2.75. Casting molds containing fresh samples were later wrapped with plastic and stored at 20oC for 24 hours. Demolded samples were subjected to 90% RH curing for 30 days inside closed plastic boxes using sprayed water. Cured samples were oven dried at 110oC for 24 hours and then subjected to a “normal atmospheric”period for two more days at 20±2oC and 60±10% RH.
The inclusion of the PM samples in this study is an attempt to understand the biodeterioration effects upon concretes made using non-conventional aggregates. It is widely accepted that Pyrite (F eS2) is the most abundant of the sulfide minerals on the Earth’s surface . Pyrite can exist in soils composed of shale, sandstone, granite and clay, which can be used as aggregates . Nowadays, the building industry